LMucko/crystallography-open-database huggingface dataset:
Synthese und Kristallstruktur von Te3 O3 (P O4)2, einer Verbindung mit fuenffach koordiniertem Tellur(IV)
Mayer, H.; Weil, M.; Zeitschrift fuer Anorganische und Allgemeine Chemie 629 (2003) 1068–1072; doi:

data_1532858
_publ_section_title
;
 Synthese und Kristallstruktur von Te3 O3 (P O4)2, einer Verbindung mit
 fuenffach koordiniertem Tellur(IV)
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              1068
_journal_page_last               1072
_journal_volume                  629
_journal_year                    2003
_chemical_formula_sum            'O11 P2 Te3'
_chemical_name_systematic        '(Te2 O3) (Te (P O4)2)'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 98.04
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   12.375
_cell_length_b                   7.317
_cell_length_c                   9.834
_cell_volume                     881.695
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            Mayer_ZAACAB_2003_1051.cif
_cod_data_source_block           O11P2Te3
_cod_original_cell_volume        881.6953
_cod_database_code               1532858
Cation size control of structure, structural fluctuations and superconductivity in L1.85 M0.15 Cu O4
McAllister, J.; Attfield, J.P.; Physical Review, Serie 3. B - Condensed Matter (18,1978-) 66 (2002) 014514-1–014514-10; doi:

data_1532859
_publ_section_title
;
 Cation size control of structure, structural fluctuations and
 superconductivity in L1.85 M0.15 Cu O4
;
_journal_name_full
'Physical Review, Serie 3. B - Condensed Matter (18,1978-)'
_journal_page_first              014514-1
_journal_page_last               014514-10
_journal_volume                  66
_journal_year                    2002
_chemical_formula_sum            'Ba0.014 Ca0.016 Cu La1.85 O4 Sr0.12'
_chemical_name_systematic        '(La0.925 Sr0.060 Ca0.008 Ba0.007)2 Cu O4'
_space_group_IT_number           64
_symmetry_space_group_name_Hall  '-A 2ab 2ab'
_symmetry_space_group_name_H-M   'A b m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.3491
_cell_length_b                   5.32404
_cell_length_c                   13.1935
_cell_volume                     375.735
_citation_journal_id_ASTM        PRBMDO
_cod_data_source_file            McAllister_PRBMDO_2002_13.cif
_cod_data_source_block           Ba0.014Ca0.016Cu1La1.85O4Sr0.12
_cod_original_cell_volume        375.7353
_cod_original_sg_symbol_Hall     '-C 2ac 2 (z,x,y)'
_cod_original_formula_sum        'Ba0.014 Ca0.016 Cu1 La1.85 O4 Sr0.12'
_cod_database_code               1532859
Cation size control of structure, structural fluctuations and superconductivity in L1.85 M0.15 Cu O4
McAllister, J.; Attfield, J.P.; Physical Review, Serie 3. B - Condensed Matter (18,1978-) 66 (2002) 014514-1–014514-10; doi:

data_1532860
_publ_section_title
;
 Cation size control of structure, structural fluctuations and
 superconductivity in L1.85 M0.15 Cu O4
;
_journal_name_full
'Physical Review, Serie 3. B - Condensed Matter (18,1978-)'
_journal_page_first              014514-1
_journal_page_last               014514-10
_journal_volume                  66
_journal_year                    2002
_chemical_formula_sum            'Ba0.076 Ca0.074 Cu La1.8 Nd0.05 O4'
_chemical_name_systematic        '(La0.9 Nd0.025 Ca0.037 Ba0.038)2 Cu O4'
_space_group_IT_number           64
_symmetry_space_group_name_Hall  '-A 2ab 2ab'
_symmetry_space_group_name_H-M   'A b m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.36154
_cell_length_b                   5.32617
_cell_length_c                   13.1752
_cell_volume                     376.237
_citation_journal_id_ASTM        PRBMDO
_cod_data_source_file            McAllister_PRBMDO_2002_14.cif
_cod_data_source_block           Ba0.076Ca0.074Cu1La1.8Nd0.05O4
_cod_original_cell_volume        376.2372
_cod_original_sg_symbol_Hall     '-C 2ac 2 (z,x,y)'
_cod_original_formula_sum        'Ba0.076 Ca0.074 Cu1 La1.8 Nd0.05 O4'
_cod_database_code               1532860
Cation size control of structure, structural fluctuations and superconductivity in L1.85 M0.15 Cu O4
McAllister, J.; Attfield, J.P.; Physical Review, Serie 3. B - Condensed Matter (18,1978-) 66 (2002) 014514-1–014514-10; doi:

data_1532861
_publ_section_title
;
 Cation size control of structure, structural fluctuations and
 superconductivity in L1.85 M0.15 Cu O4
;
_journal_name_full
'Physical Review, Serie 3. B - Condensed Matter (18,1978-)'
_journal_page_first              014514-1
_journal_page_last               014514-10
_journal_volume                  66
_journal_year                    2002
_chemical_formula_sum            'Ba0.086 Ca0.064 Cu La1.75 Nd0.1 O4'
_chemical_name_systematic        '(La0.875 Nd0.05 Ca0.032 Ba0.043)2 Cu O4'
_space_group_IT_number           56
_symmetry_space_group_name_Hall  '-P 2ab 2ac'
_symmetry_space_group_name_H-M   'P c c n'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.351
_cell_length_b                   5.3377
_cell_length_c                   13.174
_cell_volume                     376.276
_citation_journal_id_ASTM        PRBMDO
_cod_data_source_file            McAllister_PRBMDO_2002_15.cif
_cod_data_source_block           Ba0.086Ca0.064Cu1La1.75Nd0.1O4
_cod_original_cell_volume        376.2762
_cod_original_formula_sum        'Ba0.086 Ca0.064 Cu1 La1.75 Nd0.1 O4'
_cod_database_code               1532861
Cation size control of structure, structural fluctuations and superconductivity in L1.85 M0.15 Cu O4
McAllister, J.; Attfield, J.P.; Physical Review, Serie 3. B - Condensed Matter (18,1978-) 66 (2002) 014514-1–014514-10; doi:

data_1532862
_publ_section_title
;
 Cation size control of structure, structural fluctuations and
 superconductivity in L1.85 M0.15 Cu O4
;
_journal_name_full
'Physical Review, Serie 3. B - Condensed Matter (18,1978-)'
_journal_page_first              014514-1
_journal_page_last               014514-10
_journal_volume                  66
_journal_year                    2002
_chemical_formula_sum            'Ba0.094 Ca0.056 Cu La1.7 Nd0.15 O4'
_chemical_name_systematic        '(La0.85 Nd0.075 Ca0.028 Ba0.047)2 Cu O4'
_space_group_IT_number           56
_symmetry_space_group_name_Hall  '-P 2ab 2ac'
_symmetry_space_group_name_H-M   'P c c n'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.3574
_cell_length_b                   5.3338
_cell_length_c                   13.163
_cell_volume                     376.137
_citation_journal_id_ASTM        PRBMDO
_cod_data_source_file            McAllister_PRBMDO_2002_16.cif
_cod_data_source_block           Ba0.094Ca0.056Cu1La1.7Nd0.15O4
_cod_original_cell_volume        376.1367
_cod_original_formula_sum        'Ba0.094 Ca0.056 Cu1 La1.7 Nd0.15 O4'
_cod_database_code               1532862
Cation size control of structure, structural fluctuations and superconductivity in L1.85 M0.15 Cu O4
McAllister, J.; Attfield, J.P.; Physical Review, Serie 3. B - Condensed Matter (18,1978-) 66 (2002) 014514-1–014514-10; doi:

data_1532863
_publ_section_title
;
 Cation size control of structure, structural fluctuations and
 superconductivity in L1.85 M0.15 Cu O4
;
_journal_name_full
'Physical Review, Serie 3. B - Condensed Matter (18,1978-)'
_journal_page_first              014514-1
_journal_page_last               014514-10
_journal_volume                  66
_journal_year                    2002
_chemical_formula_sum            'Ba0.112 Cu La1.85 O4 Sr0.038'
_chemical_name_systematic        '(La0.925 Sr0.019 Ba0.056)2 Cu O4'
_space_group_IT_number           56
_symmetry_space_group_name_Hall  '-P 2ab 2ac'
_symmetry_space_group_name_H-M   'P c c n'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.34916
_cell_length_b                   5.34237
_cell_length_c                   13.2317
_cell_volume                     378.125
_citation_journal_id_ASTM        PRBMDO
_cod_data_source_file            McAllister_PRBMDO_2002_18.cif
_cod_data_source_block           Ba0.112Cu1La1.85O4Sr0.038
_cod_original_cell_volume        378.1248
_cod_original_formula_sum        'Ba0.112 Cu1 La1.85 O4 Sr0.038'
_cod_database_code               1532863
Cation size control of structure, structural fluctuations and superconductivity in L1.85 M0.15 Cu O4
McAllister, J.; Attfield, J.P.; Physical Review, Serie 3. B - Condensed Matter (18,1978-) 66 (2002) 014514-1–014514-10; doi:

data_1532864
_publ_section_title
;
 Cation size control of structure, structural fluctuations and
 superconductivity in L1.85 M0.15 Cu O4
;
_journal_name_full
'Physical Review, Serie 3. B - Condensed Matter (18,1978-)'
_journal_page_first              014514-1
_journal_page_last               014514-10
_journal_volume                  66
_journal_year                    2002
_chemical_formula_sum            'Ba0.136 Cu La1.776 Nd0.074 O4 Sr0.014'
_chemical_name_systematic        '(La0.888 Nd0.037 Sr0.007 Ba0.068)2 Cu O4'
_space_group_IT_number           56
_symmetry_space_group_name_Hall  '-P 2ab 2ac'
_symmetry_space_group_name_H-M   'P c c n'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.35043
_cell_length_b                   5.34393
_cell_length_c                   13.2246
_cell_volume                     378.122
_citation_journal_id_ASTM        PRBMDO
_cod_data_source_file            McAllister_PRBMDO_2002_19.cif
_cod_data_source_block           Ba0.136Cu1La1.776Nd0.074O4Sr0.014
_cod_original_formula_sum        'Ba0.136 Cu1 La1.776 Nd0.074 O4 Sr0.014'
_cod_database_code               1532864
Cation size control of structure, structural fluctuations and superconductivity in L1.85 M0.15 Cu O4
McAllister, J.; Attfield, J.P.; Physical Review, Serie 3. B - Condensed Matter (18,1978-) 66 (2002) 014514-1–014514-10; doi:

data_1532865
_publ_section_title
;
 Cation size control of structure, structural fluctuations and
 superconductivity in L1.85 M0.15 Cu O4
;
_journal_name_full
'Physical Review, Serie 3. B - Condensed Matter (18,1978-)'
_journal_page_first              014514-1
_journal_page_last               014514-10
_journal_volume                  66
_journal_year                    2002
_chemical_formula_sum            'Ba0.15 Cu La1.736 Nd0.116 O4'
_chemical_name_systematic        '(La0.868 Nd0.058 Ba0.075)2 Cu O4'
_space_group_IT_number           56
_symmetry_space_group_name_Hall  '-P 2ab 2ac'
_symmetry_space_group_name_H-M   'P c c n'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.3512
_cell_length_b                   5.34459
_cell_length_c                   13.2209
_cell_volume                     378.117
_citation_journal_id_ASTM        PRBMDO
_cod_data_source_file            McAllister_PRBMDO_2002_20.cif
_cod_data_source_block           Ba0.15Cu1La1.736Nd0.116O4
_cod_original_cell_volume        378.1173
_cod_original_formula_sum        'Ba0.15 Cu1 La1.736 Nd0.116 O4'
_cod_database_code               1532865
Studies of microstructure and ruthenium valence in the ruthenocuprates Pb2 Ru Sr2 Cu2 O8 Cl and (Ru, M) Sr2 Gd Cu2 O8 (M =Sn, Nb)
McLaughlin, A.C.; Attfield, J.P.; Liu, R.S.; Jang, L.-Y.; Zhou, W.Z.; Journal of Solid State Chemistry 177 (2004) 834–838; doi:

data_1532866
_publ_section_title
;
 Studies of microstructure and ruthenium valence in the ruthenocuprates
 Pb2 Ru Sr2 Cu2 O8 Cl and (Ru, M) Sr2 Gd Cu2 O8 (M =Sn, Nb)
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              834
_journal_page_last               838
_journal_volume                  177
_journal_year                    2004
_chemical_formula_sum            'Cl Cu2 O8 Pb2 Ru Sr2'
_chemical_name_systematic        'Pb2 Sr2 Cl (Ru Cu2 O8)'
_space_group_IT_number           127
_symmetry_space_group_name_Hall  '-P 4 2ab'
_symmetry_space_group_name_H-M   'P 4/m b m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.4671
_cell_length_b                   5.4671
_cell_length_c                   15.3674
_cell_volume                     459.319
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            McLaughlin_JSSCBI_2004_1875.cif
_cod_data_source_block           Cl1Cu2O8Pb2Ru1Sr2
_cod_original_cell_volume        459.3191
_cod_original_formula_sum        'Cl1 Cu2 O8 Pb2 Ru1 Sr2'
_cod_database_code               1532866
Crystal structures of two new oxysulfides La5 Ti2 M S5 O7 (M = Cu, Ag): evidence of anionic segregation
Meignen, V.; Cario, L.; Lafond, A.; Moelo, Y.; Meerschaut, A.; Guillot-Deudon, C.; Journal of Solid State Chemistry 177 (2004) 2810–2817; doi:

data_1532867
_publ_section_title
;
 Crystal structures of two new oxysulfides La5 Ti2 M S5 O7 (M = Cu, Ag):
 evidence of anionic segregation
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              2810
_journal_page_last               2817
_journal_volume                  177
_journal_year                    2004
_chemical_formula_sum            'Cu La5 O7 S5 Ti2'
_chemical_name_systematic        'La5 Ti2 Cu S5 O7'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   19.423
_cell_length_b                   3.9793
_cell_length_c                   18.1191
_cell_volume                     1400.424
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Meignen_JSSCBI_2004_1813.cif
_cod_data_source_block           Cu1La5O7S5Ti2
_cod_original_formula_sum        'Cu1 La5 O7 S5 Ti2'
_cod_database_code               1532867
A neutron diffraction study of Ho12 Fe32 O2
Melamud, M.; Shaked, H.; Dariel, M.P.; Journal of Applied Physics 50 (1979) 1978–1980; doi:

data_1532868
_publ_section_title
;
 A neutron diffraction study of Ho12 Fe32 O2
;
_journal_name_full               'Journal of Applied Physics'
_journal_page_first              1978
_journal_page_last               1980
_journal_volume                  50
_journal_year                    1979
_chemical_formula_sum            'Fe32 Ho12 O2'
_chemical_name_systematic        'Ho12 Fe32 O2'
_space_group_IT_number           229
_symmetry_space_group_name_Hall  '-I 4 2 3'
_symmetry_space_group_name_H-M   'I m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   8.8635
_cell_length_b                   8.8635
_cell_length_c                   8.8635
_cell_volume                     696.331
_citation_journal_id_ASTM        JAPIAU
_cod_data_source_file            Melamud_JAPIAU_1979_776.cif
_cod_data_source_block           Fe32Ho12O2
_cod_original_cell_volume        696.3309
_cod_database_code               1532868
Adsorption of chlorofluorocarbons in nanoporous solids: a combined powder neutron diffraction and computational study of C F Cl3 in NaY zeolite
Mellot-Draznieks, C.; Rodriguez-Carvajal, J.; Cox, D.E.; Cheetham, A.K.; Physical Chemistry Chemical Physics 5 (2003) 1882–1887; doi:

data_7222335
_publ_section_title
;
 Adsorption of chlorofluorocarbons in nanoporous solids: a combined powder
 neutron diffraction and computational study of C F Cl3 in NaY zeolite
;
_journal_name_full               'Physical Chemistry Chemical Physics'
_journal_page_first              1882
_journal_page_last               1887
_journal_volume                  5
_journal_year                    2003
_chemical_formula_sum
'C12.864 Al54.0096 Cl36.864 F12.864 Na47.808 O384 Si137.99'
_chemical_name_systematic        'Na54 (Al54 Si138 O384) (C F Cl3)12.87'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   24.76
_cell_length_b                   24.76
_cell_length_c                   24.76
_cell_volume                     15179.306
_citation_journal_id_ASTM        PPCPFQ
_cod_data_source_file            Mellot-Draznieks_PPCPFQ_2003_878.cif
_cod_data_source_block
Al54.0096C12.864Cl36.864F12.864Na47.808O384Si137.99
_cod_original_cell_volume        15179.31
_cod_original_formula_sum
;
Al54.0096 C12.864 Cl36.864 F12.864 Na47.808 O384 Si137.99
;
_cod_database_code               7222335
Crystal structures of R2 Pd2 Pb (R = Y, La, Ce, Pr, Nd, Sm, Gd, Tb, Dy, Ho, Er, Tm and Lu) compounds
Melnyk, G.; Tremel, W.; Kandpal, H.C.; Gulay, L.D.; Journal of Alloys Compd. 370 (2004) 217–222; doi:

data_1532869
_publ_section_title
;
 Crystal structures of R2 Pd2 Pb (R = Y, La, Ce, Pr, Nd, Sm, Gd, Tb, Dy,
 Ho, Er, Tm and Lu) compounds
;
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              217
_journal_page_last               222
_journal_volume                  370
_journal_year                    2004
_chemical_formula_sum            'Pb Pd2 Y2'
_chemical_name_systematic        'Y2 Pd2 Pb'
_space_group_IT_number           127
_symmetry_space_group_name_Hall  '-P 4 2ab'
_symmetry_space_group_name_H-M   'P 4/m b m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.7262
_cell_length_b                   7.7262
_cell_length_c                   3.6779
_cell_volume                     219.549
_citation_journal_id_ASTM        JALCEU
_cod_data_source_file            Melnyk_JALCEU_2004_1449.cif
_cod_data_source_block           Pb1Pd2Y2
_cod_original_cell_volume        219.5492
_cod_original_formula_sum        'Pb1 Pd2 Y2'
_cod_database_code               1532869
Crystal structures of R2 Pd2 Pb (R = Y, La, Ce, Pr, Nd, Sm, Gd, Tb,Dy, Ho, Er, Tm and Lu) compounds
Melnyk, G.; Kandpal, H.C.; Gulay, L.D.; Tremel, W.; Journal of Alloys Compd. 370 (2004) 217–222; doi:

data_1532870
_publ_section_title
;
 Crystal structures of R2 Pd2 Pb (R = Y, La, Ce, Pr, Nd, Sm, Gd, Tb,Dy,
 Ho, Er, Tm and Lu) compounds
;
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              217
_journal_page_last               222
_journal_volume                  370
_journal_year                    2004
_chemical_formula_sum            'La2 Pb Pd2'
_chemical_name_systematic        'La2 Pd2 Pb'
_space_group_IT_number           127
_symmetry_space_group_name_Hall  '-P 4 2ab'
_symmetry_space_group_name_H-M   'P 4/m b m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.9511
_cell_length_b                   7.9511
_cell_length_c                   3.9337
_cell_volume                     248.688
_citation_journal_id_ASTM        JALCEU
_cod_data_source_file            Melnyk_JALCEU_2004_1451.cif
_cod_data_source_block           La2Pb1Pd2
_cod_original_cell_volume        248.6885
_cod_original_formula_sum        'La2 Pb1 Pd2'
_cod_database_code               1532870
Crystal structures of R2 Pd2 Pb (R = Y, La, Ce, Pr, Nd, Sm, Gd, Tb,Dy, Ho, Er, Tm and Lu) compounds
Melnyk, G.; Kandpal, H.C.; Gulay, L.D.; Tremel, W.; Journal of Alloys Compd. 370 (2004) 217–222; doi:

data_1532871
_publ_section_title
;
 Crystal structures of R2 Pd2 Pb (R = Y, La, Ce, Pr, Nd, Sm, Gd, Tb,Dy,
 Ho, Er, Tm and Lu) compounds
;
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              217
_journal_page_last               222
_journal_volume                  370
_journal_year                    2004
_chemical_formula_sum            'Ce2 Pb Pd2'
_chemical_name_systematic        'Ce2 Pd2 Pb'
_space_group_IT_number           127
_symmetry_space_group_name_Hall  '-P 4 2ab'
_symmetry_space_group_name_H-M   'P 4/m b m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.9112
_cell_length_b                   7.9112
_cell_length_c                   3.8667
_cell_volume                     242.005
_citation_journal_id_ASTM        JALCEU
_cod_data_source_file            Melnyk_JALCEU_2004_1452.cif
_cod_data_source_block           Ce2Pb1Pd2
_cod_original_cell_volume        242.0055
_cod_original_formula_sum        'Ce2 Pb1 Pd2'
_cod_database_code               1532871
Crystal structures of R2 Pd2 Pb (R = Y, La, Ce, Pr, Nd, Sm, Gd, Tb,Dy, Ho, Er, Tm and Lu) compounds
Melnyk, G.; Kandpal, H.C.; Gulay, L.D.; Tremel, W.; Journal of Alloys Compd. 370 (2004) 217–222; doi:

data_1532872
_publ_section_title
;
 Crystal structures of R2 Pd2 Pb (R = Y, La, Ce, Pr, Nd, Sm, Gd, Tb,Dy,
 Ho, Er, Tm and Lu) compounds
;
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              217
_journal_page_last               222
_journal_volume                  370
_journal_year                    2004
_chemical_formula_sum            'Pb Pd2 Pr2'
_chemical_name_systematic        'Pr2 Pd2 Pb'
_space_group_IT_number           127
_symmetry_space_group_name_Hall  '-P 4 2ab'
_symmetry_space_group_name_H-M   'P 4/m b m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.8775
_cell_length_b                   7.8775
_cell_length_c                   3.8362
_cell_volume                     238.055
_citation_journal_id_ASTM        JALCEU
_cod_data_source_file            Melnyk_JALCEU_2004_1453.cif
_cod_data_source_block           Pb1Pd2Pr2
_cod_original_cell_volume        238.0554
_cod_original_formula_sum        'Pb1 Pd2 Pr2'
_cod_database_code               1532872
Crystal structures of R2 Pd2 Pb (R = Y, La, Ce, Pr, Nd, Sm, Gd, Tb,Dy, Ho, Er, Tm and Lu) compounds
Melnyk, G.; Kandpal, H.C.; Tremel, W.; Gulay, L.D.; Journal of Alloys Compd. 370 (2004) 217–222; doi:

data_1532873
_publ_section_title
;
 Crystal structures of R2 Pd2 Pb (R = Y, La, Ce, Pr, Nd, Sm, Gd, Tb,Dy,
 Ho, Er, Tm and Lu) compounds
;
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              217
_journal_page_last               222
_journal_volume                  370
_journal_year                    2004
_chemical_formula_sum            'Pb Pd2 Sm2'
_chemical_name_systematic        'Sm2 Pd2 Pb'
_space_group_IT_number           127
_symmetry_space_group_name_Hall  '-P 4 2ab'
_symmetry_space_group_name_H-M   'P 4/m b m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.8084
_cell_length_b                   7.8084
_cell_length_c                   3.7582
_cell_volume                     229.142
_citation_journal_id_ASTM        JALCEU
_cod_data_source_file            Melnyk_JALCEU_2004_1454.cif
_cod_data_source_block           Pb1Pd2Sm2
_cod_original_cell_volume        229.1416
_cod_original_formula_sum        'Pb1 Pd2 Sm2'
_cod_database_code               1532873